HAL Id: hal-00965628
Submitted on 25 Mar 2014
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Anharmonic suppression of charge density waves in
Maxime Leroux, Mathieu Le Tacon, Matteo Calandra, Laurent Cario, Marie
Aude Measson, Pascale Diener, Elena Borrissenko, Alexey Bosak, Pierre
To cite this version:
Maxime Leroux, Mathieu Le Tacon, Matteo Calandra, Laurent Cario, Marie Aude Measson, et al..
An-harmonic suppression of charge density waves in 2H-NbS2. Physical Review B: Condensed Matter and
Materials Physics (1998-2015), American Physical Society, 2012, 86 (15), pp.155125.
Anharmonic suppression of charge density waves in 2H-NbS2
M. Leroux,1M. Le Tacon,2M. Calandra,3L. Cario,4M-A. M´easson,5P. Diener,6E. Borrissenko,7A. Bosak,7and P. Rodi`ere1,*
1Institut N ´EEL CNRS/UJF - Grenoble, France
2Max-Planck-Institut f¨ur Festk¨orperforschung, Heisenbergstr. 1, D-70569 Stuttgart, Germany
3CNRS, Institut de Min´eralogie et de Physique des Milieux Condens´es, case 115, 4 place Jussieu, 75252 Paris Cedex 05, France 4Institut des Mat´eriaux Jean Rouxel (IMN), Universit´e de Nantes, CNRS, 2 rue de la Houssini`ere, BP3229, 44322 Nantes, France
5Laboratoire Mat´eriaux et Ph´enom`enes Quantiques, UMR 7162 CNRS, Universit´e Paris Diderot Paris 7, Bˆat. Condorcet,
75205 Paris Cedex 13, France
6SRON Netherlands Institute for Space Research - Utrecht, Netherlands 7European Synchrotron Radiation Facility - Grenoble, France
(Received 13 April 2012; revised manuscript received 2 October 2012; published 12 October 2012) The temperature dependence of the phonon spectrum in the superconducting transition-metal dichalcogenide 2H-NbS2is measured by diffuse and inelastic x-ray scattering. A deep, wide, and strongly temperature-dependent
softening of the two lowest-energy longitudinal phonon bands appears along the M symmetry line in reciprocal space. In sharp contrast to the isoelectronic compound 2H-NbSe2, the soft phonons energies are ﬁnite, even at
very low temperature, and no charge density wave instability occurs, in disagreement with harmonic ab initio calculations. We show that 2H-NbS2is at the verge of the charge density wave transition and its occurrence is
only suppressed by the large anharmonic effects. Moreover, the anharmonicity and the electron phonon coupling both show a strong in-plane anisotropy.
DOI:10.1103/PhysRevB.86.155125 PACS number(s): 78.70.Ck, 63.20.Ry, 71.45.Lr, 74.25.Kc
In transition-metal dichalcogenides (TMD) the interplay between strong electron-electron and electron-phonon inter-actions produces a wide variety of instabilities ranging from charge density wave (CDW), as in TaSe2, TaS2, NbSe2, and
TiSe2,1–3to Mott-insulating states in TaS2.4The most eminent
representative of this class of materials is 2H-NbSe2in which
a CDW (TCDW= 33 K) coexists with superconductivity (TC=
7.1 K) with a strongly anisotropic superconducting gap. The debate about the origin of the CDW instability in this system has recently been revived. Several independent studies tried to locate the CDW gap using angle-resolved photoemission spectroscopy (ARPES).5–9These studies however found either
Fermi surface nesting inconsistent with the CDW wave vector or no Fermi surface nesting at all. As such these studies were not conclusive concerning the origin of the charge density wave instability in TMD. On the other hand, theoretical calculations10,11 based on density functional theory (DFT)
reproduce the experimental CDW state, despite a real part of the bare electronic susceptibility having only a broad maximum rather than a sharp divergence. In contradiction with a pure nesting scenario, the authors conclude that the main driving force for the CDW transition is the electron-phonon coupling (EPC). The accuracy of these theoretical calculations was recently validated against experiment by direct measurements of the phonon dispersion using inelastic x-ray scattering (IXS).12
In most metallic TMD, superconductivity coexists with a charge ordered state or, at least, it occurs in proximity of such a state. For many years, it has been thought that the occur-rence of a CDW state was mandatory for superconductivity. However, there exists at least one case that disagrees with this picture, namely, 2H-NbS2. This compound is isoelectronic and
isostructural to 2H-NbSe2and has a similar superconducting
transition temperature (TC= 6 K). However, no CDW order
occurs in 2H-NbS2,13,14which does not ﬁt really well with the
variety of electronic instabilities found in the TMD family. In this work, we measure the phonon dispersion and linewidth of 2H-NbS2, using thermal diffuse scattering
(TDS) and IXS. Moreover, we perform ﬁrst-principles linear-response calculations of the harmonic phonon dispersion. Surprisingly, we ﬁnd that while theoretical calculations do predict the occurrence of a CDW state, in experiments, only a wide and marked softening of the low-energy phonon branches is present, meaning that no CDW state occurs down to 2 K. We demonstrate that this disagreement is due to the occurrence of large anharmonic effects that prevent CDW formation and stabilize the lattice. Our work shows that 2H-NbS2 is, actually, almost as close to the CDW instability
as all other metallic TMD and points out the relevance of anharmonic effects to describe the competition between CDW and superconductivity in TMD. Moreover, we show that the EPC is strongly anisotropic, giving a natural explanation to the superconducting gap anisotropy.
II. EXPERIMENTAL DETAILS
High-quality single crystals of 2H-NbS2 were prepared
by iodine vapor transport with a large excess of sulfur in a sealed quartz tube. Powder diffraction on several batches gave a predominance of 99% for 2H polytype (P 63/mmc space
group), and 1% for 3R. The polytype was then fully checked by x-ray diffraction for each selected single crystal. Reﬁned lattice parameters at room temperature are a= b = 3.33 ˚A and c= 11.95 ˚A. The superconducting properties of the main sample used for this study were published elsewhere.15,16
TDS experiments17 at 77 K and room temperature were
performed using a PILATUS 6M detector and a wavelength
λ= 0.6966 ˚A (see Fig. 1). In the (a,b) plane, the Bragg peaks are sharp: full width of the (1,1,0) reﬂection is 0.13◦,
M. LEROUX et al. PHYSICAL REVIEW B 86, 155125 (2012)
FIG. 1. Reconstruction of the x-ray diffraction in the (H,K,0) plane of 2H-NbS2 at 300 and 77 K, from a 3D mapping of thermal
diffuse scattering. A symmetrization has been applied. Diffuse intensity is present only along M and, more precisely, only where scattering geometry selects longitudinal phonons (white ellipses). No diffuse features are visible for transverse geometry (black ellipse). At 77 K, small extra spots are visible.
evidencing a good structural order. Meanwhile along the c axis, analysis of the diffraction pattern revealed a correct 2H stacking over three unit cells on average, in agreement with a previous study.18 Between the Bragg spots in the (a,b) plane, diffuse lines can be detected at room temperature, and their intensities increase at low temperature. These lines are present only along the M direction and, more precisely, only where scattering geometry selects longitudinal phonons (circled in white in Fig.1). No such diffuse features are visible for transverse polarization (circled in black in Fig.1). This indicates that an anomaly occurs for longitudinal phonons along M. In addition, at low temperature, we observe the apparition of tiny spots at wave vectors q= (0.38,0.16,0) and at the M point q= (0.5,0,0).
To get further insight regarding these diffuse features, we performed IXS measurements with a photon energy of 17.794 keV using the (9,9,9) reﬂection on the high-resolution silicon backscattering monochromator. Corresponding instru-mental energy and momentum resolutions were 2.6 meV FWHM (determined from the least-square ﬁt of the Lorentzian curve of the elastic peak), 0.017 ˚A−1in the (H,K,0) plane and 0.04 ˚A−1in the (0,0,L) direction, respectively. The x-ray beam was focused down to 200× 60 μm (width × height) on a single crystal of 2H-NbS2of 4502× 100 μm (a × b × c). We
found the tiny spots to be very weak elastic peaks, considering the high electronic susceptibility at q= (0.5,0,0), these may be traces of a charge density modulation induced by local strain or of Friedel’s oscillations. Meanwhile, the diffuse features were due to a strong phonon softening. This can be evidenced when mapping the phonon dispersion (see Fig.2) along the K and M line at fourteen different temperatures between 300 and 2 K (pumped4He cryostat). We performed
our measurements close to the (3,0,0) Bragg reﬂection, where we should observe both supposedly soft modes on LO and LA branches, according to structure factor calculations. The presence of these two modes is conﬁrmed experimentally
FIG. 2. (Color online) Experimental phonon spectrum of 2H-NbS2 at room temperature (full red circles) and 2 K (open blue
diamond), compared to ab initio, zero-temperature, and harmonic phonons (dashed lines) calculations. The two soft phonon branches along M are nearly degenerate at room temperature, and slightly split away as temperature decreases. At the exception of the scans along M at room temperature, we limited ourselves to energies below 30 meV.
by the asymmetric proﬁle of the experimental spectra in Fig.3(b). Harmonic phonon frequencies were calculated in the framework of DFT in the linear response.19We use the local
density approximation. The dynamical matrix were calculated on a 10× 10 × 1 phonon-momentum grid in the Brillouin zone and Fourier interpolated throughout the Brillouin zone. The electronic integration was performed using 20× 20 × 6 electron-momentum grid and an Hermite-Gaussian smearing (electronic temperature) Telec= 0.136 eV. The EPC
contribu-tion to the phonon linewidth (a quantity that does not depend on real or imaginary nature of the phonon frequency) has also been calculated following Ref.20. Experimental spectra were ﬁtted using standard21damped harmonic oscillator (DHO) functions
for the phonons with the Bose factor included. The linewidths were constrained to calculated electron-phonon ones (see Table I), convoluted by the quasi-Lorentzian experimental
TABLE I. Phonons linewidths γ in meV (half width at half maximum) of the ﬁrst six phonon modes, calculated ab initio for several positions along M (top) and K (bottom). Positions are expressed as a fraction x of M (respectively, K). At each position
x, the γ are sorted by increasing order of the phonon energy.
x γ1 γ2 γ3 γ4 γ5 γ6 1/5 <0.01 0.01 0.01 <0.01 0.04 0.03 2/5 0.01 <0.01 0.06 0.05 0.36 0.35 3/5 1.17 0.89 0.04 0.03 0.18 0.12 4/5 1.52 1.04 0.07 0.06 0.19 0.15 5/5 1.36 1.14 0.03 0.08 0.12 0.09 1/6 <0.01 <0.01 <0.01 <0.01 <0.01 <0.01 2/6 <0.01 <0.01 0.02 0.01 0.03 0.03 3/6 0.02 0.01 0.04 0.04 0.04 0.05 4/6 0.02 0.02 0.06 0.06 0.05 0.06 5/6 0.03 0.03 0.07 0.07 0.06 0.06 6/6 0.04 0.03 0.08 0.08 0.06 0.06 155125-2
FIG. 3. (Color online) (a) IXS scans at (H,K,L) = (3.184,−0.072,0) ﬁtted by the convolution of a DHO (with Bose factor) and the Lorentzian experimental resolution. Ab initio phonon calculations, convoluted by the experimental resolution, are in good agreement with experimental results. (b) IXS scans at (H,K,L)= (3.375,0,0) for different temperatures. For clarity, scans are shifted up. In the superimposed ﬁts, the linewidths and amplitude ratio of the two phonons are ﬁxed according to the ab initio calculations (see text). Ab initio phonon calculations, convoluted by the experimental resolution, are also in good agreement with experimental results when using higher Telec.
resolution function. This procedure yields excellent results as seen in Fig.3, and the resulting experimental dispersion of the phonons is plotted in Fig.2, together with the calculated harmonic phonon frequencies.
III. RESULTS AND DISCUSSION
Along the K direction the low-energy phonon dispersion is in excellent agreement with harmonic ﬁrst-principles calcu-lations, as also shown by the scans in Fig.3(a). On the contrary along M and close to the M point, harmonic calculations do show imaginary phonon frequencies for the lowest energy phonon modes, meaning that the high-temperature structure becomes unstable and that a CDW occurs, with ordering vector
FIG. 4. Experimental phonon energies, squared, from our ﬁtting procedure with two phonons (see text), as a function of temperature at (h,k,l)= (3.375,0,0). Energies are compatible with the mean-ﬁeld theory that predicts a power law T12. Lines are guides to the eyes.
close to 0.5a*. Experiments ﬁnd a completely different picture. Namely, a marked softening of these branches occurs but the system remains dynamically stable with no indication of CDW instabilities.
More insight can be obtained by analyzing the behavior of the measured phonon frequencies as a function of temperature. Experimentally, along the K direction (see Fig. 2) the phonon frequencies are essentially temperature independent. On the contrary, along M, and in particular close to the M point, the low-energy phonon modes are strongly temperature dependent. This is better seen in Fig.4where the lowest-energy phonon frequencies at 0.75M are plotted as a function of temperature. The phonon frequencies are more than doubled in the 2–300 K temperature range, a behavior that can only be explained by invoking strong anharmonic effects,22 as
In solids, anharmonicity has two main effects. Firstly, it is the origin of the thermal expansion in solids. However, this contribution is negligible here, as the lattice parameters barely change from zero to room temperature [a(300 K)= 3.3295 ˚A, a(2 K)= 3.3230 ˚A]. Secondly, when the lattice parameters are ﬁxed, phonon-phonon scattering results in a temperature-dependent phonon-frequency shift to higher energies and in a temperature-dependent enhancement of the phonon linewidth.22 These contributions add to the normal
electron-phonon contributions that are, on the contrary, tem-perature independent. Thus a strong temtem-perature dependence of the phonon frequencies is a ﬁngerprint of large anharmonic effects. In fact, we ﬁnd here that the square of the two phonons frequencies at the softest q vector increases linearly with temperature (see Fig.4). This power-law dependence of the frequency, also observed in 2H-NbSe2,12 is typical for a soft
mode. As temperature is increased, the unstable harmonic oscillator is stabilized by higher-order anharmonic potential, induced by the phonon-phonon interactions.23 The critical
exponent 1/2 indicates that the phonon-phonon interaction can be described in a mean-ﬁeld approach, i.e., considering the soft mode in equilibrium with the average ﬁeld induced by all other phonons.23
M. LEROUX et al. PHYSICAL REVIEW B 86, 155125 (2012) First-principles evaluation of third- and fourth-order
per-turbative coefﬁcients in phonon-phonon scattering cannot be easily done here as the harmonic solution has imaginary phonon frequencies as seen in Fig.2. As such, the anharmonic correction is as big as the bare harmonic phonon frequency itself. Nonperturbative approaches that include anharmonic effects24 are required. These approaches are, however, very time consuming and unfeasible for the case of 2H-NbS2with
six atoms per cell. In order to interpret the IXS spectra along
M, we artiﬁcially smear out the sharp Fermi surface with an electronic temperature, a technique also used in Ref.12.
We have calculated the contribution of the electron-phonon coupling to the linewidths of the phonon modes, along the two high-symmetry lines M and K. The values of the half width at half maximum are shown in TableI. Along the K direction the linewidths of the ﬁrst six branches are far below the experimental resolution (1.3 meV). However, along the
M direction, the electron-phonon coupling is responsible of a large broadening of the two soft modes on a wide range of wave vectors. In both directions, the linewidth is almost independent of the smearing of the Fermi surface, driven artiﬁcially by the increase of Telec, up to Telec= 0.34 eV and consistently with a
On the contrary, Telec has a very strong effect on the
renormalization of the phonon energies close to the M point. This is illustrated in Fig.5. Yet, a negligible renormalization is observed along the K direction, thus emphasizing the anisotropy of the electron-phonon coupling.
Typical IXS spectra calculated at 0.75M for electronic temperatures of Telec= 0.34 and 0.27 eV (including the
electron-phonon linewidth, weakly dependent on the chosen electronic temperature, as well as the experimental resolution) are shown in Fig. 3(b) and are in good agreement with the experimental data. The electronic temperature smears the Fermi surface, and by doing so suppresses the effect of the EPC. This in turn increases the phonon frequency artiﬁcially and stabilizes the lattice. However, this increase of Telecis not the correct physical picture, since to reproduce
FIG. 5. Calculated phonon energy squared for the two lowest branches at 0.8M as a function of the smearing of the Fermi surface with Telec.
changes in spectra in the 0–300 K temperature range, the electronic temperature must be changed by at least 0.1 eV, and even more in the case of 2H-NbSe212or 1T-TiSe2.25Thus
considering this effect as the origin of the temperature behavior of the phonon frequencies is incorrect.12,25
On the contrary, the aforementioned anharmonicity, ne-glected in these ﬁrst-principles calculations, is likely respon-sible for these discrepancies. This was already suggested by Varma and Simons,26 who demonstrated that anharmonicity
can be responsible for a reduction by an order of magnitude of TCDW in 1T-TaS2, hence accounting for the anomalously
large ratio of the CDW gap amplitude to TCDW in these
compounds. The strong mean-ﬁeld power law temperature dependence of the soft phonon modes of 2H-NbS2, and
the prediction by harmonic DFT calculations of a CDW instability close to the M point, both consistently indicate that anharmonic effects are, in this case, so strong that they actually suppress the CDW and stabilize the crystal structure, leaving, however, the superconducting properties essentially unaffected.27
In real space, the main components of the soft phonon modes are the vibrations of the Nb atoms in the (a,b) plane, but also the vibrations along the c axis of a couple of S atoms situated just above and below the plane of Nb atoms. The longitudinal displacement of Nb atoms along M corresponds to a movement toward this couple of S atoms. Interestingly, the distance between these S atoms is unusually short (2.97 ˚A, while typical S-S bond are 3.3–3.4 ˚A28). It therefore suggests that the displacement of Nb atoms is hampered by the great elastic cost of moving apart the S atoms, which would be the microscopic origin of the anharmonicity. The decisive role of the force constant between the S atoms in the same S-Nb-S sandwich was already emphasized in a study based on a tight-binding approach29and with ﬁrst-principles calculations in TiSe2.30 In this respect, 2H-NbS2 is rather unique as it is
on the verge of the CDW transition and is only stabilized by anharmonic effects.
A second important result of our work is that the EPC (responsible for the softening close to the M point) is strongly anisotropic throughout the Brillouin zone. The ab initio calculation yields a very large phonon linewidth of 1.5 meV at 0.8 M, due to the EPC, compared to less than 0.1 meV along the K line. This strong in-plane anisotropy has necessarily important consequences for the superconducting properties of TMD. In this respect, it is instructive to compare superconduct-ing gap measurements of the two isoelectronic dichalcogenides 2H-NbSe2and 2H-NbS2. In the former, there exists two main
values of the superconducting gap.31–35 This was initially
attributed to the CDW order, presumably competing with the superconducting instability.7,9,36,37 However, a similar observation in the superconducting state of 2H-NbS2 by
the same various methods (scanning tunneling spectroscopy, speciﬁc heat measurements, Hc1, magnetic penetration depth
measurement), clearly ruled out this assumption.13,15,16,38 As
a consequence of the strongly anisotropic softening of the phonons that we report in this study, the EPC, and therefore the pairing strength, are themselves highly anisotropic. This sug-gests that the two superconducting gap amplitudes observed in 2H-NbS2, and by extension in 2H-NbSe2, rather originate
from the anisotropy of the electron-phonon coupling. 155125-4
In conclusion, we identiﬁed two wide soft phonon modes in 2H-NbS2. They strongly soften along the M direction as
the temperature is lowered, but their energies always remain ﬁnite and never freeze into a static modulation of the lattice. This absence of a CDW is in disagreement with the ﬁrst-principles harmonic calculations. The mean-ﬁeld power-law temperature dependence over the range 300–2 K is also an unambiguous evidence of strong anharmonic effects which smear the effect of the EPC. These anharmonic effects are responsible for the absence of CDW in 2H-NbS2, but also
for the low TCDWtransition temperatures in other TMD. Thus
2H-NbS2, which is the lightest compound among the TMD, is
a TMD on the verge of a CDW, only hampered by anharmonic effects. These, however, leave the superconducting properties
essentially unaffected compared to 2H-NbSe2, which suggests
that the relevant parameters for superconductivity in TMD are the anisotropy and strength of the electron-phonon coupling, rather than the nature of the ground state.
M. Leroux greatly acknowledges L. P. Gor’kov for a long and fruitful correspondence. We thank D. Gambetti for technical assistance. Fruitful discussions with P. Monceau, M. Krisch, and X. Blase are also gratefully acknowledged. Experiments were carried out at the European Synchrotron Radiation Facility, on beamlines ID28 (IXS) and ID29 (TDS). Calculations were performed at the IDRIS supercomputing center (Proposal No. 091202).
*Corresponding author: firstname.lastname@example.org
1E. Morosan, H. W. Zandbergen, B. S. Dennis, J. W. G. Bos,
Y. Onose, T. Klimczuk, A. P. Ramirez, N. P. Ong, and R. J. Cava,
Nat. Phys. 2, 544 (2006).
2H. Cercellier, C. Monney, F. Clerc, C. Battaglia, L. Despont,
M. G. Garnier, H. Beck, P. Aebi, L. Patthey, H. Berger, and L. Forr´o,Phys. Rev. Lett. 99, 146403 (2007).
3A. F. Kusmartseva, B. Sipos, H. Berger, L. Forr´o, and E. Tutis, Phys. Rev. Lett. 103, 236401 (2009).
4B. Sipos, A. F. Kusmartseva, A. Akrap, H. Berger, L. Forro, and
E. Tutis,Nat. Mater. 7, 960 (2008) .
5K. Rossnagel, O. Seifarth, L. Kipp, M. Skibowski, D. Voß,
P. Kr¨uger, A. Mazur, and J. Pollmann,Phys. Rev. B 64, 235119 (2001).
6T. Valla, A. V. Fedorov, P. D. Johnson, P.-A. Glans, C. McGuinness,
K. E. Smith, E. Y. Andrei, and H. Berger,Phys. Rev. Lett. 92, 086401 (2004).
7T. Kiss, T. Yokoya, A. Chainani, S. Shin, T. Hanaguri, M. Nohara,
and H. Takagi,Nat. Phys. 3, 720 (2007).
8D. W. Shen, Y. Zhang, L. X. Yang, J. Wei, H. W. Ou, J. K. Dong,
B. P. Xie, C. He, J. F. Zhao, B. Zhou, M. Arita, K. Shimada, H. Namatame, M. Taniguchi, J. Shi, and D. L. Feng,Phys. Rev. Lett. 101, 226406 (2008).
9S. V. Borisenko, A. A. Kordyuk, V. B. Zabolotnyy, D. S. Inosov,
D. Evtushinsky, B. B¨uchner, A. N. Yaresko, A. Varykhalov, R. Follath, W. Eberhardt, L. Patthey, and H. Berger,Phys. Rev. Lett. 102, 166402 (2009).
10M. D. Johannes, I. I. Mazin, and C. A. Howells,Phys. Rev. B 73, 205102 (2006).
11M. Calandra, I. I. Mazin, and F. Mauri,Phys. Rev. B 80, 241108 (2009).
12F. Weber, S. Rosenkranz, J.-P. Castellan, R. Osborn, R. Hott,
R. Heid, K.-P. Bohnen, T. Egami, A. H. Said, and D. Reznik,Phys. Rev. Lett. 107, 107403 (2011).
13I. Guillam´on, H. Suderow, S. Vieira, L. Cario, P. Diener, and
P. Rodi`ere,Phys. Rev. Lett. 101, 166407 (2008).
14M. Naito and S. Tanaka,J. Phys. Soc. Jpn. 51, 219 (1982). 15J. Kacmarcik, Z. Pribulova, C. Marcenat, T. Klein, P. Rodi`ere,
L. Cario, and P. Samuely, Phys. Rev. B 82, 014518 (2010).
16P. Diener, M. Leroux, L. Cario, T. Klein, and P. Rodi`ere,Phys. Rev. B 84, 054531 (2011).
17A. Bosak, M. Krisch, D. Chernyshov, B. Winkler, V. Milman,
K. Refson, and C. Schulze-Briese,Z. Kristall. 227, 84 (2012). 18H. Katzke,Z. Kristall. 217, 127 (2002).
19P. Giannozzi et al.,J. Phys.: Condens. Matter 21, 395502 (2009). 20P. B. Allen,Phys. Rev. B 6, 2577 (1972).
21B. F˚ak and B. Dorner,Physica B 234, 1107 (1997).
22M. Calandra, M. Lazzeri, and F. Mauri, Physica C: Superconductivity 456, 38 (2007).
23J. F. Scott,Rev. Mod. Phys. 46, 83 (1974).
24I. Errea, B. Rousseau, and A. Bergara,Phys. Rev. Lett. 106, 165501 (2011).
25F. Weber, S. Rosenkranz, J.-P. Castellan, R. Osborn, G. Karapetrov,
R. Hott, R. Heid, K.-P. Bohnen, and A. Alatas,Phys. Rev. Lett. 107, 266401 (2011).
26C. M. Varma and A. L. Simons,Phys. Rev. Lett. 51, 138 (1983). 27K. Nasu,Phys. Rev. B 44, 7625 (1991).
28F. Jellinek, G. Brauer, and H. Muller,Nature (London) 185, 376 (1960).
29Y. Nishio, M. Shirai, N. Suzuki, and K. Motizuki,J. Phys. Soc. Jpn. 63, 156 (1994).
30M. Calandra and F. Mauri,Phys. Rev. Lett. 106, 196406 (2011). 31P. Garoche, J. Veyssi´e, P. Manuel, and P. Molini´e, Solid State
Commun. 19, 455 (1976).
32H. F. Hess, R. B. Robinson, R. C. Dynes, J. M. Valles, and J. V.
Waszczak,Phys. Rev. Lett. 62, 214 (1989).
33R. Corcoran, P. Meeson, Y. Onuki, P.-A. Probst, M. Springford,
K. Takita, H. Harima, G. Y. Guo, and B. L. Gyorffy, J. Phys.: Condens. Matter 6, 4479 (1994).
34D. Sanchez, A. Junod, J. Muller, H. Berger, and F. L´evy,Physica B 204, 167 (1995).
35I. Guillam´on, H. Suderow, F. Guinea, and S. Vieira,Phys. Rev. B 77, 134505 (2008).
36J. D. Fletcher, A. Carrington, P. Diener, P. Rodi`ere, J. P. Brison,
R. Prozorov, T. Olheiser, and R. W. Giannetta,Phys. Rev. Lett. 98, 057003 (2007).
37A. H. Castro Neto,Phys. Rev. Lett. 86, 4382 (2001).
38M. Leroux, P. Rodi`ere, L. Cario, and T. Klein,Physica B 407, 1813 (2012).